Your SlideShare is downloading.
×

×
Saving this for later?
Get the SlideShare app to save on your phone or tablet. Read anywhere, anytime – even offline.

Text the download link to your phone

Standard text messaging rates apply

Like this presentation? Why not share!

- An Introduction to Crystallography by Hassan Harraz 2751 views
- Crystal structures & Packing Fraction by bagga1212 34871 views
- What Is Crystallography? by RiAus 1521 views
- Crystal systems by institute of adva... 3684 views
- Space lattice and crystal structure... by Manmeet Singh 2135 views
- Crystallography by nandanrocker 196 views
- Introduction to Crystallography by Kalai Vanan 544 views
- Crystallography and X ray Diffracti... by Nakkiran Arulmozhi 948 views
- Crystalography by md5358dm 1284 views
- Crystalography by Anshul Chauhan 501 views
- TOF-SIMS Machine and software. by Alger_P 578 views
- BT631-14-X-Ray_Crystallography_Crys... by Rajesh G 303 views

1,036

Published on

Crystallography and structure

Crystallography and structure

No Downloads

Total Views

1,036

On Slideshare

0

From Embeds

0

Number of Embeds

3

Shares

0

Downloads

94

Comments

0

Likes

3

No embeds

No notes for slide

- 1. Crystal StructureCrystal Structure Means: PERIODIC ARRANGEMENT OF ATOMS/IONS OVER LARGE ATOMIC DISTANCES Leads to structure displaying LONG-RANGE ORDER that is Measurable and Quantifiable All metals, many ceramics, and some polymers exhibit this “High Bond Energy” and a More Closely Packed Structure CRYSTAL STRUCTURES Devesh agrawal
- 2. Amorphous MaterialsAmorphous Materials These less densely packed lower bond energy “structures” can be found in Metals are observed in Ceramic GLASS and many “plastics” Materials Lacking Long range order
- 3. Crystal Systems – Some Definitional information 7 crystal systems of varying symmetry are known These systems are built by changing the lattice parameters: a, b, and c are the edge lengths α, β, and γ are interaxial angles Fig. 3.4, Callister 7e. Unit cell: smallest repetitive volume which contains the complete lattice pattern of a crystal.
- 4. A crystal’s unit cell dimensions are defined by six numbers, the lengths of the 3 axes, a, b, and c, and the three interaxial angles, α, β and γ. Unit cell is the smallest unit of a crystal, which, if repeated, could generate the whole crystal. Crystals are made of infinite number of unit cells
- 5. A crystal lattice is a 3-D stack of unit cells Crystal lattice is an imaginative grid system in three dimensions in which every point (or node) has an environment that is identical to that of any other point or node.
- 6. Crystal Systems Crystal structures are divided into groups according to unit cell geometry (symmetry).
- 7. Crystal Forms 6 large groups of crystal systems: • (1) CUBIC • (2) TETRAGONAL • (3) ORTHORHOMBIC • (4) HEXAGONAL • (5) MONOCLINIC • (6) TRICLINIC CRYSTALLOGRAPHIC AXES • During the process of crystallization, crystals assume various geometric shapes dependent on the ordering of their atomic structure and the physical and chemical conditions under which they grow. • These forms may be subdivided, using geometry, into six systems.
- 8. (1) CUBIC (aka ISOMETRIC) The three crystallographic axes a1, a2, a3 (or a, b, c) are all equal in length and intersect at right angles (90 degrees) to each other. (2) TETRAGONAL Three axes, all at right angles, two of which are equal in length (a and b) and one (c) which is different in length (shorter or longer). Note: If c was equal in length to a or b, then we would be in the cubic system!
- 9. (4) HEXAGONAL Four axes! Three of the axes fall in the same plane and intersect at the axial cross at 120 degrees between the positive ends. These 3 axes, labeled a1, a2, and a3, are the same length. The fourth axis, termed c, may be longer or shorter than the a axes set. The c axis also passes through the intersection of the a axes set at right angle to the plane formed by the a set. (3) ORTHORHOMBIC Three axes, all at right angles, and all three of different lengths. Note: If any axis was of equal length to any other, then we would be in the tetragonal system!
- 10. (6) TRICLINIC The three axes are all unequal in length and intersect at three different angles (any angle but 90 degrees). Note: If any two axes crossed at 90 degrees, then we would be describing a monoclinic crystal! (5) MONOCLINIC Three axes, all unequal in length, two of which (a and c) intersect at an oblique angle (not 90 degrees), the third axis (b) is perpendicular to the other two axes. Note: If a and c crossed at 90 degrees, then we would be in the orthorhombic system!
- 11. Lattices  In 1848, Auguste Bravais demonstrated that in a 3-dimensional system there are fourteen possible lattices  A Bravais lattice is an infinite array of discrete points with identical environment  seven crystal systems + four lattice centering types = 14 Bravais lattices  Lattices are characterized by translation symmetry Auguste Bravais (1811-1863)
- 12. Crystal Structure of Metals – of engineering interest
- 13. • Rare due to low packing density (only Po – Polonium -- has this structure) • Close-packed directions are cube edges. • Coordination No. = 6 (# nearest neighbors) for each atom as seen (Courtesy P.M. Anderson) Simple Cubic Structure (SC)
- 14. • APF for a simple cubic structure = 0.52 APF = a3 4 3 π (0.5a) 31 atoms unit cell atom volume unit cell volume Atomic Packing Factor (APF) APF = Volume of atoms in unit cell* Volume of unit cell *assume hard spheres Adapted from Fig. 3.23, Callister 7e. close-packed directions a R=0.5a contains (8 x 1/8) = 1 atom/unit cell Here: a = Rat*2 Where Rat is the ‘handbook’ atomic radius
- 15. • Coordination # = 8 Adapted from Fig. 3.2, Callister 7e. (Courtesy P.M. Anderson) • Atoms touch each other along cube diagonals within a unit cell. --Note: All atoms are identical; the center atom is shaded differently only for ease of viewing. Body Centered Cubic Structure (BCC) ex: Cr, W, Fe (α), Tantalum, Molybdenum 2 atoms/unit cell: (1 center) + (8 corners x 1/8)
- 16. Atomic Packing Factor: BCC a APF = 4 3 π ( 3a/4)32 atoms unit cell atom volume a3 unit cell volume length = 4R = Close-packed directions: 3 a • APF for a body-centered cubic structure = 0.68 a R Adapted from Fig. 3.2(a), Callister 7e. a2 a3
- 17. • Coordination # = 12 Adapted from Fig. 3.1, Callister 7e. (Courtesy P.M. Anderson) • Atoms touch each other along face diagonals. --Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing. Face Centered Cubic Structure (FCC) ex: Al, Cu, Au, Pb, Ni, Pt, Ag 4 atoms/unit cell: (6 face x ½) + (8 corners x 1/8)
- 18. • APF for a face-centered cubic structure = 0.74 Atomic Packing Factor: FCC The maximum achievable APF! APF = 4 3 π ( 2a/4)34 atoms unit cell atom volume a3 unit cell volume Close-packed directions: length = 4R = 2 a Unit cell contains: 6 x1/2 + 8 x1/8 = 4 atoms/unit cella 2 a Adapted from Fig. 3.1(a), Callister 7e. (a = 2√2*R)
- 19. • Coordination # = 12 • ABAB... Stacking Sequence • APF = 0.74 • 3D Projection • 2D Projection Adapted from Fig. 3.3(a), Callister 7e. Hexagonal Close-Packed Structure (HCP) 6 atoms/unit cell ex: Cd, Mg, Ti, Zn • c/a = 1.633 (ideal) c a A sites B sites A sites Bottom layer Middle layer Top layer
- 20. We find that both FCC & HCP are highest density packing schemes (APF = .74) – this illustration shows their differences as the closest packed planes are “built-up”
- 21. Theoretical Density, ρ where n = number of atoms/unit cell A = atomic weight VC = Volume of unit cell = a3 for cubic NA = Avogadro’s number = 6.023 x 1023 atoms/mol Density = ρ = VC NA n A ρ = CellUnitofVolumeTotal CellUnitinAtomsofMass
- 22. • Ex: Cr (BCC) A = 52.00 g/mol R = 0.125 nm n = 2 ∴ a = 4R/√3 = 0.2887 nm a R ρ = a3 52.002 atoms unit cell mol g unit cell volume atoms mol 6.023x1023 Theoretical Density, ρ ρtheoretical ρactual = 7.18 g/cm3 = 7.19 g/cm3
- 23. Locations in Lattices: Point Coordinates Point coordinates for unit cell center are a/2, b/2, c/2 ½ ½½ Point coordinates for unit cell (body diagonal) corner are 111 Translation: integer multiple of lattice constants  identical position in another unit cell z x y a b c 000 111 y z • 2c • • • b b
- 24. Crystallographic Directions 1. Vector is repositioned (if necessary) to pass through the Unit Cell origin. 2. Read off line projections (to principal axes of U.C.) in terms of unit cell dimensions a, b, and c 3. Adjust to smallest integer values 4. Enclose in square brackets, no commas [uvw] ex: 1, 0, ½ => 2, 0, 1 => [201] -1, 1, 1 families of directions <uvw> z x Algorithm where ‘overbar’ represents a negative index [111]=> y
- 25. What is this Direction ????? Projections: Projections in terms of a,b and c: Reduction: Enclosure [brackets] x y z a/2 b 0c 1/2 1 0 1 2 0 [120]
- 26. ex: linear density of Al in [110] direction a = 0.405 nm Linear Density – considers equivalance and is important in Slip  Linear Density of Atoms ≡ LD = a [110] Unit length of direction vector Number of atoms # atoms length 1 3.5 nm a2 2 LD − == # atoms CENTERED on the direction of interest! Length is of the direction of interest within the Unit Cell
- 27. Determining Angles Between Crystallographic Direction: ( ) ( ) 1 1 2 1 2 1 2 2 2 2 2 2 2 1 1 1 2 2 2 u u v v w w Cos u v w u v w θ −   + + =  + + • + +   Where ui’s , vi’s & wi’s are the “Miller Indices” of the directions in question – also (for information) If a direction has the same Miller Indices as a plane, it is NORMAL to that plane
- 28. HCP Crystallographic Directions 1. Vector repositioned (if necessary) to pass through origin. 2. Read off projections in terms of unit cell dimensions a1, a2, a3, or c 3. Adjust to smallest integer values 4. Enclose in square brackets, no commas [uvtw] [1120]ex: ½, ½, -1, 0 => Adapted from Fig. 3.8(a), Callister 7e. dashed red lines indicate projections onto a1 and a2 axes a1 a2 a3 -a3 2 a 2 2 a 1 -a3 a1 a2 z Algorithm
- 29. HCP Crystallographic Directions  Hexagonal Crystals  4 parameter Miller-Bravais lattice coordinates are related to the direction indices (i.e., u'v'w') in the ‘3 space’ Bravais lattice as follows. = = = 'ww t v u )vu( +- )'u'v2( 3 1 - )'v'u2( 3 1 -= ]uvtw[]'w'v'u[ → Fig. 3.8(a), Callister 7e. -a3 a1 a2 z
- 30. Computing HCP Miller- Bravais Directional Indices (an alternative way): -a3 a1 a2 z We confine ourselves to the bravais parallelopiped in the hexagon: a1-a2- Z and determine: (u’,v’w’) Here: [1 1 0] - so now apply the models to create M-B Indices ( ) ( ) ( ) ( ) ( ) ( ) 1 1 12 ' ' 2 1 1 1 3 3 3 1 1 12 ' ' 2 1 1 1 3 3 3 1 1 2 2 3 3 3 ' 0 M-B Indices: [1120] u u v v v u t u v w w = − = ∗ − = → = − = ∗ − = → = − + = − + = − → − = =
- 31. Defining Crystallographic Planes  Miller Indices: Reciprocals of the (three) axial intercepts for a plane, cleared of fractions & common multiples. All parallel planes have same Miller indices.  Algorithm (in cubic lattices this is direct) 1. Read off intercepts of plane with axes in terms of a, b, c 2. Take reciprocals of intercepts 3. Reduce to smallest integer values 4. Enclose in parentheses, no commas i.e., (hkl) → families {hkl}
- 32. Crystallographic Planes -- families
- 33. Crystallographic Planes z x y a b c 4. Miller Indices (110) example a b c z x y a b c 4. Miller Indices (100) 1. Intercepts 1 1 ∞ 2. Reciprocals 1/1 1/1 1/∞ 1 1 0 3. Reduction 1 1 0 1. Intercepts 1/2 ∞ ∞ 2. Reciprocals 1/½ 1/∞ 1/∞ 2 0 0 3. Reduction 2 0 0 example a b c
- 34. Crystallographic Planes z x y a b c • • • 4. Miller Indices (634) example 1. Intercepts 1/2 1 3/4 a b c 2. Reciprocals 1/½ 1/1 1/¾ 2 1 4/3 3. Reduction 6 3 4 (001)(010), Family of Planes {hkl} (100), (010),(001),Ex: {100} = (100),
- 35. x y z Intercepts Intercept in terms of lattice parameters Reciprocals Reductions Enclosure ∝a -b c/2 ∝ -1 1/2 0 -1 2 N/A (012) Determine the Miller indices for the plane shown in the sketch
- 36. Crystallographic Planes (HCP)  In hexagonal unit cells the same idea is used example a1 a2 a3 c 4. Miller-Bravais Indices (1011) 1. Intercepts 1 ∞ -1 1 2. Reciprocals 1 1/∞ 1 0 -1 -1 1 1 3. Reduction 1 0 -1 1 a2 a3 a1 z Adapted from Fig. 3.8(a), Callister 7e.
- 37. Crystallographic Planes  We want to examine the atomic packing of crystallographic planes – those with the same packing are equivalent and part of families  Iron foil can be used as a catalyst. The atomic packing of the exposed planes is important. a) Draw (100) and (111) crystallographic planes for Fe. b) Calculate the planar density for each of these planes.
- 38. Planar Density of (100) Iron Solution: At T < 912°C iron has the BCC structure. (100) Radius of iron R = 0.1241 nm R 3 34 a = 2D repeat unit =Planar Density = a2 1 atoms 2D repeat unit = nm2 atoms 12.1 m2 atoms = 1.2 x 1019 1 2 R 3 34area 2D repeat unit Atoms: wholly contained and centered in/on plane within U.C., area of plane in U.C.
- 39. Polymorphism: Also in Metals  Two or more distinct crystal structures for the same material (allotropy/polymorphism) titanium α (HCP), β(BCC)-Ti carbon: diamond, graphite BCC FCC BCC 1538ºC 1394ºC 912ºC δ-Fe γ-Fe α-Fe liquid iron system:
- 40. (a) An exploded view of the graphite (C) unit cell. (From F. H. Norton, Elements of Ceramics, 2nd ed., Addison-Wesley Publishing Co., Inc., Reading, MA, 1974.) (b) A schematic of the nature of graphite’s layered structure. (From W. D. Kingery, H. K. Bowen, and D. R. Uhlmann, Introduction to Ceramics, 2nd ed., John Wiley & Sons, Inc., NY, 1976.)
- 41. Densities of Material Classes ρmetals > ρceramics > ρpolymers Why? Data from Table B1, Callister 7e. ρ(g/cm)3 Graphite/ Ceramics/ Semicond Metals/ Alloys Composites/ fibers Polymers 1 2 20 30 *GFRE, CFRE, & AFRE are Glass, Carbon, & Aramid Fiber-Reinforced Epoxy composites (values based on 60% volume fraction of aligned fibers in an epoxy matrix).10 3 4 5 0.3 0.4 0.5 Magnesium Aluminum Steels Titanium Cu,Ni Tin, Zinc Silver, Mo Tantalum Gold, W Platinum Graphite Silicon Glass -soda Concrete Si nitride Diamond Al oxide Zirconia HDPE, PS PP, LDPE PC PTFE PET PVC Silicone Wood AFRE* CFRE* GFRE* Glass fibers Carbon fibers Aramid fibers Metals have... • close-packing (metallic bonding) • often large atomic masses Ceramics have... • less dense packing • often lighter elements Polymers have... • low packing density (often amorphous) • lighter elements (C,H,O) Composites have... • intermediate values In general
- 42. • Single Crystals -Properties vary with direction: anisotropic. -Example: the modulus of elasticity (E) in BCC iron: • Polycrystals -Properties may/may not vary with direction. -If grains are randomly oriented: isotropic. (Epoly iron = 210 GPa) -If grains are textured, anisotropic. 200 µm Source of data is R.W. Hertzberg, Deformation and Fracture Mechanics of Engineering Materials, 3rd ed., John Wiley and Sons, 1989. courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD]. Single vs Polycrystals E (diagonal) = 273 GPa E (edge) = 125 GPa
- 43. Effects of Anisotropy:
- 44. • Atoms may assemble into crystalline or amorphous structures. • We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP). SUMMARY • Common metallic crystal structures are FCC, BCC, and HCP. Coordination number and atomic packing factor are the same for both FCC and HCP crystal structures. • Crystallographic points, directions and planes are specified in terms of indexing schemes. Crystallographic directions and planes are related to atomic linear densities and planar densities.
- 45. • Some materials can have more than one crystal structure. This is referred to as polymorphism (or allotropy). SUMMARY • Materials can be single crystals or polycrystalline. Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but are generally non-directional (i.e., they are isotropic) in polycrystals with randomly oriented grains. • X-ray diffraction is used for crystal structure and interplanar spacing determinations.

Be the first to comment